Discussion Chain ID: 134772
================================================================================

User asked: Home made PCB tinning solution

By reviewing a couple of [articles](https://www.pcbway.com/blog/Engineering_Technical/Tin_Plating_Copper_PC_Boards.html) and [videos](https://hackaday.com/2017/10/23/tinning-solution-from-the-hardware-store/) I decided to give some try to develop a PCB tinning solution at home. Based on most of the articles, the easiest way to develop this solution is by using the following chemicals: * _Stannous Chloride_ ($\ce{SnCl2}$) * _Thiourea_ ($\ce{CH4N2S}$) * _Sulfuric Acid_ ($\ce{H2SO4}$) After checking with a couple of stores, I noticed that _Thiourea_ is not available to buy in any of the stores. Now my questions are: 1. What _Thiourea_ does in this solution? 2. Is there any substitute available for _Thiourea_ (for this process)? 3. Is it possible to prepare _Thiourea_ from any other chemicals? ([It seems using _Ammonium Thiocyanate_ ($\ce{NH4SCN}$) can do that job](https://www.prepchem.com/synthesis-of-thiourea/), but it looks like a lengthy and complex process to do at home.) 4. Is there any possible way to build a tinning solution without using _Thiourea_?

Discussion:
Comment: According to [this](https://www.ourpcb.com/pcb-tinning.html), thiourea is essential to tinning. Yet, silver polishing contains thiourea so follow them and see what happens. Good luck.
Comment: Also keep in mind that thiourea is a human carcinogen. No wonder you cannot find it.

Answer 1 (2 votes):
Thiourea ($\ce{(H2N)2C=S}$) is a very important component of tinning solution because tinning is a redox process. That's because thiourea is a powerful reducing agent (Ref.1), chemically and biochemically used in redox reactions _in vitro_ or _in vivo_ : $$\ce{(H2N)2C=S <=> (H2N)2C-S-S-C(NH2)2 + 2e-} \quad E^\circ = \pu{0.418 V} \tag1$$ The oxidizing agent in this process is $\ce{Sn^2+}$ ion, which reduces it self during the process: $$\ce{Sn^2+ + 2e- <=> Sn} \quad E^\circ = \pu{-0.1375 V} \tag2$$ As a result, following redox reaction happens: $$\ce{(H2N)2C=S + Sn^2+ <=> (H2N)2C-S-S-C(NH2)2 + Sn} \quad E_\mathrm{rxn}^\circ = \pu{0.2805 V} \tag3$$ Since $E_\mathrm{rxn}^\circ $ is positive, the reaction is spontanious in standard conditions and no electric current is necessary. When you dip your circuit in the solution (or touch surface to surface of the solution), metallic tin would deposit as a thin layer. As an alternative to $\ce{(H2N)2C=S}$, dimethylated or diethylated thiourea can be used in those reactions, which require electrode potential within the range of $\pu{0.418 V}$ or higher (Ref.2): $$\ce{(CH3NH)2C=S <=> (CH3NH)2C-S-S-C(NHCH3)2 + 2e-} \quad E^\circ = \pu{0.460 V} \tag4$$ $$\ce{(C2H5NH)2C=S <=> (C2H5NH)2C-S-S-C(NHC2H5)2 + 2e-} \quad E^\circ = \pu{0.450 V} \tag5$$ In tanning process, theoretically, any component with oxidative potential bigger than $\pu{-0.1375 V}$ can be used as the reluctant. Thus, best alternative come to my mind is ascorbic acid (Vitamin C). Recently, natural source of ascorbic acid source, extract of fruits of _Averrhoa bilimbi_ (Sinhala name: _Billin_), has been used to prepare silver and gold nanoparticles from corresponding salts (Ref.3): [](https://i.sstatic.net/11zo4.jpg) In any event ascorbic acid didn't work, there is a way to synthesize thiourea derivatives without using thiocyanate or isocyanate. The scheme is illustrated in the bottom box of above diagram (Ref.4). The $E^\circ$ of these derivatives should be closer to that depicted in equations $(4)$ and $(4)$. However, any attemp to synthesize these compound should be done in certified chemical laboratory under the observation of an experienced chemist. Keep in mind that thiourea is a potent carcinogen. **Note:** It is well known that _silver polishing_ reagents contain thiourea ($50\%$ by weight; Ref.5). You may able to extract thiourea from such solutions. * * * **References:** 1. Paul W. Preisler, Louis Berger, “Oxidation-Reduction Potentials of Thiol-Dithio Systems: Thiourea-Formamidine Disulfide,” _J. Am. Chem. Soc._ **1947** , _69(2)_ , 322–325 (<https://doi.org/10.1021/ja01194a048>). 2. Paul W. Preisler, “Oxidation--Reduction Potentials of Thiol--Disulfide Systems. III. Substituted Thioureas and Compounds Containing Two Thioureido Groups,” _J. Am. Chem. Soc._ **1949** , _71(8)_ , 2849–2852 (<https://doi.org/10.1021/ja01176a076>). 3. R. S. Rimal Isaac, G. Sakthivel, Ch. Murthy, “Green Synthesis of Gold and Silver Nanoparticles Using _Averrhoa bilimbi_ Fruit Extract,” _Journal of Nanotechnology_ **2013** , _Article ID 906592_ , 6 pages (<https://doi.org/10.1155/2013/906592>). 4. Wei Tan, Jianpeng Wei, Xuefeng Jiang, “Thiocarbonyl Surrogate via Combination of Sulfur and Chloroform for Thiocarbamide and Oxazolidinethione Construction,” _Org. Lett._ **2017** , _19(8)_ , 2166–2169 (<https://doi.org/10.1021/acs.orglett.7b00819>). 5. Mark Laing, Mark Beeston, "Silver polish formulation containing thiourea," _US Patent_ 5,958,854, 1999 (Application No.: 08/869,685 in 1997).


================================================================================

